Upcoming SlideShare
×

# 7 stress & strain curves

4,759 views

Published on

1 Comment
5 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• thanks for the ppt

Are you sure you want to  Yes  No
Views
Total views
4,759
On SlideShare
0
From Embeds
0
Number of Embeds
18
Actions
Shares
0
174
1
Likes
5
Embeds 0
No embeds

No notes for slide

### 7 stress & strain curves

1. 1. STRESS-STRAIN CURVES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 August 23, 2001 Introduction Stress-strain curves are an extremely important graphical measure of a material’s mechanical properties, and all students of Mechanics of Materials will encounter them often. However, they are not without some subtlety, especially in the case of ductile materials that can undergo sub- stantial geometrical change during testing. This module will provide an introductory discussion of several points needed to interpret these curves, and in doing so will also provide a preliminary overview of several aspects of a material’s mechanical properties. However, this module will not attempt to survey the broad range of stress-strain curves exhibited by modern engineering materials (the atlas by Boyer cited in the References section can be consulted for this). Several of the topics mentioned here — especially yield and fracture — will appear with more detail in later modules. “Engineering” Stress-Strain Curves Perhaps the most important test of a material’s mechanical response is the tensile test1, in which one end of a rod or wire specimen is clamped in a loading frame and the other subjected to a controlled displacement δ (see Fig. 1). A transducer connected in series with the specimen provides an electronic reading of the load P(δ) corresponding to the displacement. Alternatively, modern servo-controlled testing machines permit using load rather than displacement as the controlled variable, in which case the displacement δ(P) would be monitored as a function of load. The engineering measures of stress and strain, denoted in this module as σe and e respec- tively, are determined from the measured the load and deﬂection using the original specimen cross-sectional area A0 and length L0 as σe = P A0 , e = δ L0 (1) When the stress σe is plotted against the strain e, an engineering stress-strain curve such as that shown in Fig. 2 is obtained. 1 Stress-strain testing, as well as almost all experimental procedures in mechanics of materials, is detailed by standards-setting organizations, notably the American Society for Testing and Materials (ASTM). Tensile testing of metals is prescribed by ASTM Test E8, plastics by ASTM D638, and composite materials by ASTM D3039. 1
2. 2. Figure 1: The tension test. Figure 2: Low-strain region of the engineering stress-strain curve for annealed polycrystaline copper; this curve is typical of that of many ductile metals. In the early (low strain) portion of the curve, many materials obey Hooke’s law to a reason- able approximation, so that stress is proportional to strain with the constant of proportionality being the modulus of elasticity or Young’s modulus, denoted E: σe = E e (2) As strain is increased, many materials eventually deviate from this linear proportionality, the point of departure being termed the proportional limit. This nonlinearity is usually as- sociated with stress-induced “plastic” ﬂow in the specimen. Here the material is undergoing a rearrangement of its internal molecular or microscopic structure, in which atoms are being moved to new equilibrium positions. This plasticity requires a mechanism for molecular mo- bility, which in crystalline materials can arise from dislocation motion (discussed further in a later module.) Materials lacking this mobility, for instance by having internal microstructures that block dislocation motion, are usually brittle rather than ductile. The stress-strain curve for brittle materials are typically linear over their full range of strain, eventually terminating in fracture without appreciable plastic ﬂow. Note in Fig. 2 that the stress needed to increase the strain beyond the proportional limit in a ductile material continues to rise beyond the proportional limit; the material requires an ever-increasing stress to continue straining, a mechanism termed strain hardening. These microstructural rearrangements associated with plastic ﬂow are usually not reversed 2